Latex Hydraulic Cement Latex Hydraulic Cement Additives D. GERRY WALTERS This paper describes...
Embed Size (px)
Transcript of Latex Hydraulic Cement Latex Hydraulic Cement Additives D. GERRY WALTERS This paper describes...
TRANSPORTATION RESEARCH RECORD 1204 71
Latex Hydraulic Cement Additives
D. GERRY WALTERS
This paper describes latexes used to modify hydraulic cement mixes. It includes definitions and brief descriptions of the his· tory, chemistry, types, and production oflatexes, together with an explanation of how latex modifies hydraulic cement and discusses the problems and advantages associated with' such systems.
What is a latex? As reported in the literature (1), an accepted definition is
a dispersion of organic polymer particles in water. But this really doesn't tell you very much. What does it
look like? What is an organic polymer? Most latexes or latices are milky fluids that are generally white to off-white in color. Their consistency can vary from very fluid to very viscous.
What is meant by an organic polymer? This can be defined as a substance that is composed of giant
molecules and that has been formed by the union of a con- siderable number of simple molecules, usually many tens of thousands.
The simple molecules are known as monomers and the reaction that combines them is called polymerization. The polymer may be a homopolymer if it is made by the poly- merization of one monomer, or a copolymer when two or more monomers are polymerized.
The first reference to latex was in the early 16th century when the Spanish explorers reported that the South American Indians were making rubber footwear by standing in latex that was obtained from trees. That tree, known as Hevea brasilienis, produces latex naturally, which, of course, is known as natural rubber latex (NRL).
Seedlings of those trees were transferred from South Amer- ~ca to Europe; and from Europe, a few were taken to Malaya m the Far East. From those few seedlings, huge plantations and a large industry have grown. The latex, obtained from the tree by a process known as tapping, may be concentrated to be sold as latex or coagulated and dried to be sold as rubber. Production of natural rubber latex in Malaya for 1984 exceeded 200,000 metric tons.
Natural rubber latex is a dispersion of polyisoprene (a homopolymer) that i.s polymerized and formed into a latex by the tree. Incidentally, NRL has been, and in some places continues to be, used in conjunction with hydraulic cements. In 1924, a patent was granted to Lefebure for the combined use of NRL and cement (2).
Until early in the 20th century, the only available latex was natural rubber latex; then synthetic latexes started to appear on the scene.
Since World War II, there has been a tremendous increase
Emulsion Polymers Division, Reichhold Chemicals, Inc., Dover, Del. 19901.
in the number and type of synthetic polymer latexes that have been made and are commercially available.
The following is a list of the majority of latex types used with hydraulic cements today:
• Styrene-butadiene copolymers (S-B) • Poly acrylic esters (PAE) • Styrene-acrylic copolymers (S-A) • Vinyl acetate homopolymers (PV A) • Vinyl acetate-ethylene copolymers (V AE) • Vinyl acetate-acrylic copolymers (V AC) • Vinyl acetate-vinyl ester of versatic acid copolymers (VA-
This list is not all inclusive. Many other types of latexes are made, probably have been tested, and possibly are being used with hydraulic cements. Some of the latexes listed above are used with hydraulic cements other than portland; and in some cases, the mixes do not contain any aggregate. For this reason, they are referred to as additives rather than the more usual term, admixtures.
All of the latexes listed above are manufactured by a proc- ess known as emulsion polymerization and therefore are sometimes referred to as emulsions.
The basic process involves mixing the monomer(s) with water, a stabilizer, and an initiator. The initiator generates a free radical that causes the monomer(s) to polymerize by chain addition.
An example of chain addition polymerization is given in Figure 1. The free radical reacts with a molecule of butadiene (or styrene), and the resultant molecule further reacts with a molecule of styrene (or butadiene). This chain of molecules continues to grow until the free radical either no longer con- tacts a suitable molecule or contacts a chemical that "absorbs" it.
A typical recipe for emulsion polymerization is given in Figure 2. The usual method of polymerization is to charge the water, the stabilizers, the other ingredients, and part of the monomer(s) to the reactor under agitation. The temper- ature is increased to a desired point, then the initiator system is fed to the reactor followed by the remainder of the mon- omer(s) . By temperature control and possibly other chemical additions, the reaction is normally taken to a 90 to 99 percent conversion. Excess monomer(s) are reduced to acceptable levels by a process known as stripping.
The resultant latex may be concentrated or diluted, and small levels of materials such as preservatives and stabilizers may be added. Many other ingredients are used in polymer- ization; they are incorporated for a myriad of reasons, such as controlling pH, particle size, and molecular weight.
Many, many latexes are on the market, but about 95 percent of them are not suitable for use with hydraulic cements.
1. Free Radical & Butadiene
Ro + CH2=CH-CH=CH2 -> CH2-CH=CH-CH2• R
2. Copolymerizalion with Styrene
FIGURE 1 Free radical polymerization of butadiene and styrene (J).
Latexes can be divided into three classes according to the type of electrical charge on the particle, which is determined by the type of stabilizers: cationic (positively charged), anionic (negatively charged), and nonionic (no charge). In general, cationic or anionic latexes are not suitable for use with hydraulic cements because they lack the necessary stability. Most latexes used with portland cement are stabilized primarily with non- ionic stabilizers. Typical recipes for some of the latexes used with portland cement are given in Figures 3, 4, and 5.
The preservatives added to the latex after polymerization usually provide protection against bacteria contamination and give improved aging resistance . Sometimes additional stabi- lizers are added to provide more stability. Also, defoam or antifoam agents may be added to reduce air entrainment when the latex is mixed with the cement and aggregates.
PRINCIPLE OF LATEX MODIFICATION
Classical theories on the principle of latex modification of hydraulic cement concrete and mortars have appeared in the literature (J, 4). Latex modification is governed by two proc- esses: cement hydration and latex film formation. Generally the cement hydration process precedes the film formation (5), except at surfaces where loss of water by evaporation causes the latex film to form faster than the cement hydrates. It is believed that a co-matrix phase, which consists of the cement gel and latex polymer, is formed as the binder for the mix.
The process of forming the polymer film from the latex is usually referred to as coalescence'.
When latex is mixed with fresh cement mortar or concrete, the organic polymer particles are uniformly dispersed in the cement paste . In such latex-cement paste, the cement gel is gradually formed by cement hydration . With water loss due to the development of the cement gel structure and to evap- oration, the polymer particles of the latex are gradually confined in the capillary pores.
As cement hydration and evaporation loss continue, the capillary water is reduced and the polymer particles flocculate
Other Ingredients 0.0
FIGURE 2 Typical recipe for emulsion polymerization (J).
TRANSPORTATION RESEARCH RECORD 1204
Parts by Weight
Partially hydrolyzed polyvinyl alcohol 6.0
Hydrogen peroxide 35%
Sodium formaldehyde sulfoxylate
FIGURE 3 Vinyl acetate homopolymer latex (J).
to form a continuous close-packed layer on the surfaces of the cement gel-unhydrated cement particle mixtures. These layers simultaneously adhere to the mixtures and the silicate layer of the aggregate surfaces. One should bear in mind that the size of the pores in the cement paste ranges from a few angstroms to several thousand angstroms; whereas the par- ticle size of latexes typically used with cement ranges from 500 to 5,000 angstroms (6). Ultimately, with water loss by cement hydration and evaporation, the close-packed polymer particles on the cement hydrates coalesce into continuous films or membranes .
These films or membranes bind the cement hydrates together, resulting in a monolithic network in which polymer films inter- penetrate the cement-hydrate phase. Such a structure acts as the co-matrix phase for latex-modified mortar and concrete, with the aggregates being bound by such a matrix.
It is generally considered that unmodified hardened cement paste is predominantly an agglomerated structure of calcium silicate hydrates and calcium hydroxide bound together by relatively weak van der Waal's forces. Consequently, micro- cracks occur easily in such a paste under stress, leading tO the low tensile strength and fracture toughness of ordinary cement mortar and concrete.
By contrast,in la